210R-93 Erosion of Concrete in Hydraulic Structures
Embed Size (px)
Transcript of 210R-93 Erosion of Concrete in Hydraulic Structures
Erosion of Concrete in Hydraulic Structures
Reported by ACI Committee 210
James R. GrahamChairman
Patrick J. CreeganWallis S. HamiltonJohn G. Hendrickson, Jr.Richard A. Kaden
James E. McDonaldGlen E. NobleErnest K. Schrader
Committee 210 recognizes with thanks the contributions of Jeanette M. Ballentine, J. Floyd Best, Gary R. Mass, William D. McEwen, Myron B. Petrowsky,Melton J. Stegall, and Stephen B. Tatro.
Members of ACI Committee 210 voting on the revisions:
Stephen B. TatroChairman
Patrick J. Creegan Angel E. HerreraJames R. Graham Richard A
James E. McDonald
This report outlines the causes, control, maintenance, and repair of erosion in hydraulic structures. Such erosion occurs from three major causes: cavi-ration, abrasion, and chemical attack. Design parameters, materials selec-tion and quality,environmental factors, and other issues affecting the per-formance of concrete are discussed.
Evidence exists to suggest that given the operating characteristics andconditions to which a hydraulic structure will be subjected, it can be de-signed to mitigate future erosion of the concrete. However,operationalfactors change or are not clearly known and hence erosion of concrete sur-faces occurs and repairs must follow. This report briefly treats the subjectof concrete erosion and repair and provides numerous references to de-tailed treatment of the subject.
Keywords: abrasion; abrasion resistance; aeration; cavitation; chemical attackconcrete dams; concrete pipes; corrosion; corrosion resistance; deterioration;erosion; grinding (material removal): high-strength concretes; hydraulic struc- tures; maintenance; penstocks; pipe linings; pipes (tubes); pitting polymerconcrete; renovating; repairs; spillways; tolerances (mechanics); wear.
PART 1-CAUSES OF EROSIONChapter 1-Introduction, pg. 210R-2
ACI Committee Reports, Guides, Standard Practices, andCommentaries are intended for guidance in designing, plan-ning, executing, or inspecting construction and in preparingspecifications. References to these documents shall not bemade in the Project Documents. If items found in thesedocuments are desired to be a part of the Project Docu-ments, they should be phrased in mandatory language andincorporated into the Project Documents.
. Kaden Ernest K. Schrader
Chapter 2-Erosion by cavitation, pg. 210R-22.1-Mechanism of cavitation2.2-Cavitation index2.3-Cavitation damage
Chapter 3-Erosion by abrasion, pg. 210R-53.1-General3.2-Stilling basin damage3.3-Navigation lock damage3.4-Tunnel lining damage
Chapter 4-Eros ion by chemical attack, 4.1-Sources of chemical attack
4.2-Erosion by mineral-free water4.3-Erosion by miscellaneous causes
PART 2-CONTROL OF EROSIONChapter 5-Control of cavitation erosion, pg. 210R-8
5.1-Hydraulic design principles5.2-Cavitation indexes for damage and construction
tolerances5. 3-Using aeration to control damage
ACI 210 R-93 supersedes ACI 210 R-87 and became effective September 1,1993.Minor revisions have been made to the report. Year designations have beenremoved from recommended references to make the current edition the re-ferenced version.
Copyright Q 1987, American Concrete Institute.All rights reserved including righs of reproduction and use in any form or by
any means, including the making of copies by any photo process, or by any elect-tronic or mechanical device printed, written, or oral, or recording for sound orvisual reproduction or for we in any knowledge or retrieval system or device,unless permission in writing is obtained from the copyright proprietors.
210R-2 ACI COMMITTEE REPORT
5.4-Fatigue caused by vibration5.5-Materials5.6-Materials testing5.7-Construction practices
Chapter 6-Control of abrasion erosion, pg. 210R-146.1-Hydraulic considerations6.2-Material evaluation6.3-Materials
Chapter 7-Control of erosion by chemical attack, pg.210R-15
7.1-Control of erosion by mineral-free water7.2-Control of erosion from bacterial action7.3-Control of erosion by miscellaneous chemical
PART3-MAINTENANCE AND REPAIR OF EROSIONChapter 8-Periodic inspections and corrective action,pg. 21OR-17
8.l-General8.2-Inspection program8.3-Inspection procedures8.4-Reporting and evaluation
Chapter 9-Repair methods and materials, pg. 210R-189.1-Design considerations9.2-Methods and materials
Chapter 1O-References, pg. 210R-21l0.l-Specified and/or recommended references10.2-Cited references
Appendix-Notation, pg. 210R-24
PART I-CAUSES OF EROSIONCHAPTER 1-INTRODUCTION
Erosion is defined in this report as the progressive dis-integration of a solid by cavitation, abrasion, or chemicalaction. This report is concerned with: 1) cavitation ero-sion resulting from the collapse of vapor bubbles formedby pressure changes within a high-velocity water flow; 2)abrasion erosion of concrete in hydraulic structurescaused by water-transported silt, sand, gravel, ice, ordebris; and 3) disintegration of the concrete in hydraulicstructures by chemical attack. Other types of concretedeterioration are outside the scope of this report.
Ordinarily, concrete in properly designed, constructed,used, and maintained hydraulic structures will undergoyears of erosion-free service. However, for a variety ofreasons including inadequate design or construction, oroperational and environmental changes, erosion does oc-cur in hydraulic structures. This report deals with threemajor aspects of such concrete erosion:
Part 1 discusses the three major causes of concreteerosion in hydraulic structures: cavitation, abrasion, andchemical attack.
Part 2 discusses the options available to the designerand user to control concrete erosion in hydraulic struc-tures.
Part 3 discusses the evaluation of erosion problemsand provides information on repair techniques. Part 3 isnot comprehensive, and is intended as a guide for theselection of a repair method and material.
CHAPTER 2-EROSION BY CAVITATION
2.1-Mechanism of cavitationCavitation is the formation of bubbles or cavities in a
liquid. In hydraulic structures, the liquid is water, and thecavities are filled with water vapor and air. The cavitiesform where the local pressure drops to a value that willcause the water to vaporize at the prevailing fluid tem-perature. Fig. 2.1 shows examples of concrete surface ir-regularities which can trigger formation of these cavities.The pressure drop caused by these irregularities is gen-erally abrupt and is caused by local high velocities andcurved streamlines. Cavities often begin to form nearcurves or offsets in a flow boundary or at the centers ofvortices.
When the geometry of flow boundaries causes stream-lines to curve or converge, the pressure will drop in thedirection toward the center of curvature or in the direc-tion along the converging streamlines. For example, Fig.2.2 shows a tunnel contraction in which a cloud of cavi-ties could start to form at Point c and then collapse at
F L O W ,-Vopar cavities - /Vapor cavities
A O F F S E T INTO F L O W 8. OFFSET AWAY FROM FLOW
-flapor cavities - ,Vopor cavities
C A B R U P T C U R V A T U R EAWAY FROM FLOW
D . A B R U P T S L O P EA W A Y F R O M F L O W
~Er cavities - /apor cavities
E . V O I D O R T R A N S V E R S E
G R 0 0 V EF. R O U G H E N E D S U R F A C E
I /- DamageP R O T R U D I N G J O I N T
Fig. 2.1-Cavitation situations at surface irregularities
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 21OR-3
Fig. 2.2-Tunnel contraction
Point d. The velocity near Point c is much higher thanthe average velocity in the tunnel upstream, and thestreamlines near Point c are curved. Thus, for propervalues of flow rate and tunnel pressure at 0, the localpressure near Point c will drop to the vapor pressure ofwater and cavities will occur. Cavitation damage is pro-duced when the vapor cavities collapse. The collapsesthat occur near Point d produce very high instantaneouspressures that impact on the boundary surfaces and causepitting, noise, and vibration. Pitting by cavitation isreadily distinguished from the worn appearance causedby abrasion because cavitation pits cut around the hardercoarse aggregate particles and-have irregular and roughedges.
2.2-Cavitation indexThe cavitation index is a dimensionless measure used
to characterize the susceptibility of a system to cavitate.Fig. 2.2 illustrates the concept of the cavitation index. Insuch a system, the critical location for cavitation is atPoint c.
The static fluid pressure at Location 1 will be
where p, is the absolute static pressure at Point c; y isthe specific weight of the fluid (weight per unit volume);z, is the elevation at Point c; and zg is the elevation at 0.
The pressure drop in the fluid as it moves along astreamline from the reference Location 0 to Location 1will be
PO - IPC + Y @C - %>I
wherepO is the static pressure at 0.The cavitation index normalizes this pressure drop to
the dynamic pressure ‘/z p vo2
u=I+) - [PC + Y (2, - z,)l
- Eq. (2-l)‘/2 p v;
where p is the density of the fluid (mass per unit vol-ume) and v0 is the fluid velocity at 0.
Readers familiar with the field of fluid mechanics mayrecognize the cavitation index as a special form of theEuler number or pressure coefficient, a matter discussed
in Rouse (1978).If cavitation is just beginning and there is a bubble of
vapor at Point c, the pressure in the fluid adjacent to thebubble is approximately the pressure within the bubble,which is the vapor pressure pv of the fluid at the fluid’stemperature.
Therefore, the pressure drop along the streamlinefrom 0 to 1 required to produce cavitation at the crownis
and the cavitation index at the conditioncavitation is
It can be deduced from fluid mechanics considerations(Knapp, Daily, and Hammitt 1970) - and confirmed ex-perimentally - that in a given system cavitation willbegin at a specific Us, no matter which combination ofpressure and velocity yields that uc.
If the system operates at a u above uc, the system doesnot cavitate. If u is below a=, the lower the value of a,the more severe the cavitation action in a given system.Therefore, the designer should insure that the operatingu is safely above uc for the system’s critical location.
Actual values of uc for different systems differ mark-edly, depending on the shape of flow passages, the shapeof objects fixed in the flow, and the location wherereference pressure and velocity are measured.
For a smooth surface with slight changes of slope inthe direction of flow, the value of uc may be below 0.2.For systems that produce strong vortices, uc may exceed10. Values of uc for various geometries are given inChapter 5. Falvey (1982) provides additional informationon predicting cavitation in spillways.
Since, in theory, a system having a given geometry willhave a certain a,- despite differences in scale, uc is auseful concept in model studies. Tullis (1981) describesmodeling of cavitation in closed circuit flow. Cavitationconsiderations (such as surface tension) in scaling frommodel to prototype are discussed in Knapp, Daily, andHammitt (1970) and Arndt (1981).
2.3-Cavitation damageCavitation bubbles will grow and travel with the flow-
ing water to an area where the pressure field will causecollapse. Cavitation damage can begin at that point.When a cavitation bubble collapses or implodes close toor against a solid surface, an extremely high pressure isgenerated, which acts on an infinitesimal area of the sur-face for a very short time period. A succession of thesehigh-energy impacts will damage almost any solid mater-ial. Tests on soft metal show initial cavitation damage inthe form of tiny craters. Advanced stages of damage show
21OR-4 AC1 COMMITTEE REPORT
an extremely rough honeycomb texture with some holesthat penetrate the thickness of the metal. This type ofpitting often occurs in pump impellers and marine pro-pellers.
The progression of cavitation erosion in concrete isnot as well documented as it is in metals. For bothclasses of material, however, the erosion progressesrapidly after an initial period of exposure slightlyroughens the surface with tiny craters or pits. Possible
explanations are that: a) the material immediately be-neath the surface is more vulnerable to attack; b) thecavitation impacts are focused by the geometry of thepits themselves; or c) the structure of the material hasbeen weakened by repeated loading (fatigue). In anyevent, the photograph in Fig. 2.3 clearly shows a ten-dency for the erosion to follow the mortar matrix andundermine the aggregate. Severe cavitation damage willtypically form a Christmas-tree configuration on spillwaychute surfaces downstream from the point of origin asshown in Fig. 2.4.
Fig. 2.3-Cavitation erosion of intakelock at point of tunnel contraction
wall of a navigation
Fig. 2.4-``Christmas tree” configuration of cavitationdamage on a high-head tunnel surface
Microfissures in the surface and between the mortarand coarse aggregate are believed to contribute to cavi-tation damage. Compression waves in the water that fillssuch interstices may produce tensile stresses which causemicrocracks to propagate. Subsequent compression wavescan then loosen pieces of the material. The simultaneouscollapse of all of the cavities in a large cloud, or thesupposedly slower collapse of a large vortex, quite pro-bably is capable of suddenly exerting more than 100 at-mospheres of pressure on an area of many square inches.Loud noise and structural vibration attest to-the violenceof impact. The elastic rebounds from a sequence of suchblows may cause and propagate cracks and otherdamage, causing chunks of material to break loose.
Fig. 2.5 shows the progress of erosion of concretedownstream from two protruding bolts used to generatecavitation. The tests were made at a test facility locatedat Detroit Dam, Oregon. Fig. 2.6 shows cavitationdamage on test panels after 47 hours of exposure tohigh-velocity flows in excess of 100 ft per second (ft/sec)[40 meters per second (m/sec) ]. A large amount of cavita-tion erosion caused by a small offset at the upstreamedge of the test slab is evident.
test slab fe aturing cavitation
Fig. 2.7 shows severe cavitation damage that occurredto the flip bucket and training walls of an outlet structureat Lucky Peak Dam, Idaho. In this case, water velocitiesof 120 ft/sec (37 m/sec) passed through a gate structureinto an open outlet manifold, part of which is shownhere. Fig. 2.8 shows cavitation damage to the side of abaffle block and the floor in the stilling basin atYellowtail Afterbay Dam, Montana.
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 210R-5
Fig. 2.6-Cavitation erosion pattern after 47 hours of testingat a 240 ft velocity head
Fig. 2.7-Cavitation erosion of discharge outlet trainingwall and flip bucket
Fig. 2.8-Cavitation erosion of baffle block and floor instilling basin
Once erosion has begun, the rate of erosion may beexpected to increase because protruding pieces of aggre-gate become new generators of vapor cavities. In fact, acavity cloud often is caused by the change in direction of
the boundary at the downstream rim of an eroded de-pression. Collapse of this cloud farther downstream startsa new depression, and so on, as indicated in Fig. 2.4.
Once cavitation damage has substantially altered theflow regime, other mechanisms then begin to act on thesurface. These, fatigue due to vibrations of the mass, in-clude high water velocities striking the irregular surfaceand mechanical failure due to vibrating reinforcing steel.Significant amounts of material may be removed by theseadded forces, thereby accelerating failure of the struc-ture. This sequence of cavitation damage followed byhigh-impact damage from the moving water was clearlyevident in the 1983 spillway tunnel failure at Glen Can-yon Dam, Arizona.
CHAPTER 3-EROSION BY ABRASION
3.1-GeneralAbrasion erosion damage results from the abrasive
effects of waterborne silt, sand, gravel, rocks, ice, andother debris impinging on a concrete surface duringoperation of a hydraulic structure. Abrasion erosion. isreadily recognized by the smooth, worn-appearing con-crete surface, which is distinguished from the small holesand pits formed by cavitation erosion, as can be com-pared in Fig. 2.8 and 3.1. Spillway aprons, stilling basins,sluiceways, drainage conduits or culverts, and tunnellinings are particularly susceptible to abrasion erosion.
The rate of erosion is dependent on a number of fac-tors including the size, shape, quantity, and hardness ofparticles being transported, the velocity of the water, andthe quality of the concrete. While high-quality concreteis capable of resisting high water velocities for manyyears with little or no damage, the concrete cannot with-stand the abrasive action of debris grinding or repeatedlyimpacting on its surface. In such cases, abrasion erosionranging in depth from a few inches (few centimeters) toseveral feet (a meter or more) can result depending onthe flow conditions. Fig. 3.2 shows the relationship be-tween fluid-bottom velocity and the size. of particleswhich that velocity can transport.
Fig. 3.1-Abrasion damage to concrete baffle blocks andfloor area in Yellowtail Diversion Dam sluiceway, Montana
210R-6 ACI COMMITTEE REPORT
Particle Diameter , in.
0.01 .02 .04 .06 .08 0.1 . 2 .4 .6 .88 1.0 2 4 6 8 10 2 0 40I 1 I I I I I I I I I I I I I I I
8 0 - - 24
60- - I8
4 for Vb in ft/S and d in in.:
Vb’ 2.72 dg I
ifor Vb in m/S ond d in mm:
for Vb in ft/s and d in in:
for vb in m/ss and d in mm:
Graph based on"The Start of Bed-Load Movement and- .24the Relation Between Competent Bottom Velocities in .18a Channel and the Transportable Sediment Size" M.S.
Thesiss by N.K. Berry, Colorado University, 1948. _ .12
. 2 - - .06
0. I I I III I I I I I I I I I I I I I.2 .4 .6 .8 1.0 ; 4 6 8 IO 20 40 60 80 100 2 0 0 400 600 800
Particle Diameter d, mm
Fig. 3.2-Bottom velocity versus transported sediment size
3.2-Stilling basin damageA typical stilling basin design includes a downstream
sill from 3 to 20 ft (1 to 6 m) high intended to create apermanent pool to aid in energy dissipation of high-velo-city flows. Unfortunately, in many cases these pools alsotrap rocks and debris (Fig. 3.3). The stilling basins atLibby and Dworshak Dams, high-head hydroelectricstructures, were eroded to maximum depths of approxi-mately 6 and 10 ft (2 and 3 m), respectively. In the lattercase, nearly 2000 yd3 (1530 m3) of concrete and bedrockwere eroded from the stilling basin (Fig. 3.4). Impact
forces associated with turbulent flows carrying large rocksand boulders at high velocity contribute to the surfacedamage of concrete.
Fig. 3.3-Typical debris resulting from abrasion erosion of concrete
Fig. 3.4-Erosion of stilling basin flooor slab, Dworshak Dam
There are many cases where the concrete in outletworks stilling basins of low-head structures has also ex-hibited abrasion erosion. Chute blocks and baffles withinthe basin are particularly susceptible to abrasion erosionby direct impact of waterborne materials. There also havebeen several cases where baffle blocks connected to thebasin training walls have generated eddy currents behindthese baffles, resulting in significant localized damage to
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 210R-7
the stilling basin walls and floor slab, as shown in Fig.3.5.
Fig. 3.5-Abrasion erosion damage to stilling basin, NolinDam
In most cases, abrasion erosion damage in stillingbasins has been the result of one or more of the follow-ing: a) construction diversion flows through constrictedportions of the stilling basin, b) eddy currents created bydiversion flows or powerhouse discharges adjacent to thebasin, c) construction activities in the vicinity of thebasin, particularly those involving cofferdams; d) nonsym-metrical discharges into the basin; e) separation of flowand eddy action within the basin sufficient to transportriprap from the exit channel into the basin; f) failure toclean basins after completion of construction work, andg) topography of the outflow channel (McDonald 1980).
3.3-Navigation lock damageHydraulic structures other than spillways are also
subject to abrasion erosion damage. When Upper St. An-thony Falls navigation lock was dewatered to repair adamaged miter gate, an examination of the filling andemptying laterals and discharge laterals revealed con-siderable abrasion erosion (Fig. 3.6). This erosion of the
concrete to maximum depths of 23 in. (580 mm) wascaused by rocks up to 18 in. (460 mm) in diameter, whichhad entered the laterals, apparently during discharge ofthe flood of record through the lock chamber. Subse-quent filling and emptying of the lock during normaloperation agitated those rocks, causing them to erode theconcrete by grinding.
Fig. 3.6-Abrasion erosion damage to discharge lateral:Upper St. Anthony Falls Lock
3.4-Tunnel lining damageConcrete tunnel linings are susceptible to abrasion
erosion damage, particularly when the water carries largequantities of sand, gravel, rocks, and other debris. Therehave been many instances where the concrete in bothtemporary and permanent diversion tunnels has experi-enced abrasion erosion damage. Generally, the tunnelfloor or invert is the most heavily damaged. Wagner(1967) has described the performance of Glen CanyonDam diversion tunnel outlets.
CHAPTER 4-EROSION BY CHEMICAL ATTACK
4.1-Sources of chemical attackThe compounds present in hardened portland cement
are attacked by water and by many salt and acid solu-tions; fortunately, in most hydraulic structures, thedeleterious action on a mass of hardened portlandcement concrete with a low permeability is so slow it isunimportant. However, there are situations where chemi-cal attack can become serious and accelerate deteriora-tion and erosion of the concrete.
Acidic environments can result in deterioration ofexposed concrete surfaces. The acidic environment mayrange from low acid concentrations found in mineral-freewater to high acid concentrations found in many proces-sing plants. Alkali environments can also cause concretedeterioration. In the presence of moisture, alkali soilscontaining sulfates of magnesium, sodium, and calciumattack concrete, forming chemical compounds whichimbibe water and swell, and can damage the concrete.
Hydrogen sulfide corrosion, a form of acid attack, iscommon in septic sanitary systems. Under certain con-ditions this corrosion can be very severe and cause earlyfailure of a sanitary system.
4.2-Erosion by mineral-free waterHydrated lime is one of the compounds formed when
cement and water combine. It is readily dissolved bywater and more aggressively dissolved by pure miner-al-free water, found in some mountain streams. Dissolvedcarbon dioxide is contained in some fresh waters in suf-ficient quantity to make the water slightly acidic and addto its aggressiveness. Scandinavian countries havereported serious attacks by fresh water, both on exposedconcrete surfaces and interior surfaces of conduits whereporosity or cracks have provided access. In the UnitedStates, there are many instances where the surface of theconcrete has been etched by fresh water flowing over it,
210R-8 ACI COMMITTEE REPORT
but serious damage from this cause is uncommon (Hol-land et al. 1980). This etching is particularly evident athydraulic structures carrying runoff from high mountainstreams in the Rocky Mountains and the Cascade Moun-tains of the central and western United States. A survey(ICOLD 1951) of the chemical composition of raw waterin many reservoirs throughout the United States indicatesa nearly neutral acid-alkaline balance (pH) for most ofthese waters.
4.3-Erosion by miscellaneous causes4.3.1 Acidic environments-Decaying vegetation is the
most frequent source of acidity in natural waters. Decom-position of certain minerals may be a source of acidity insome localities. Running water that has a pH as low as6.5 will leach lime from concrete, reducing its strengthand making it more porous and less resistant to freezingand thawing and other chemical attack. The amount oflime leached from concrete is a function of the area ex-posed and the volume of concrete. Thin, small-diameterdrains will deteriorate in a few years when exposed tomildly acidic waters, whereas thick pipe and massivestructures will not be damaged significantly for manyyears under the same exposure, provided the cover overthe reinforcing steel meets normal design standards.
Waters flowing from peat beds may have a pH as lowas 5. Acid of this strength will aggressively attackconcrete, and for this reason, when conveyances forground water are being designed, the aggressiveness ofthe water should be tested to determine its compatibilitywith the concrete. This is particularly true in pressureconduits.
4.3.2 Bacterial action - M o s t of the literature addres-sing the problem of deterioration of concrete resultingfrom bacterial action has evolved because of the greatimpact of this corrosive mechanism on concrete sewersystems. This is a serious problem which, as Rigdon andBeardsley (1958) observed, occurs more readily in warmclimates such as California, USA; Australia; and SouthAfrica. This problem also occurs at the terminus of longpumped sewage force mains in the northern climates(Pomeroy 1974).
Sulfur-reducing bacteria belong to the genus of bac-teria that derives the energy for its life processes fromthe reduction of some element other than carbon, suchas nitrogen, sulfur, or iron (Rigdon and Beardsley 1958).Some of these bacteria are able to reduce the sulfatesthat are present in natural waters and produce hydrogensulfide as a waste product. These bacteria, as stated byWetzel (1975), are anaerobic.
Another group of bacteria takes the reduced sulfurand oxidizes it back so that sulfuric acid is formed. Thegenus Thiobacillus is the sulfur-oxidizing bacteria that ismost destructive to concrete. It has a remarkable toler-ance to acid. Concentrations of sulfuric acid as great as5 percent do not completely inhibit its activity.
Sulfur-oxidizing bacteria are likely to be foundwherever warmth, moisture, and reduced compounds of
sulfur are present. Generally, a free water surface isrequired, in combination with low dissolved oxygen insewage and low velocities that permit the buildup ofscum on the walls of a pipe in which the anaerobic sul-fur-reducing bacteria can thrive. Certain conditions mustprevail before the bacteria can produce hydrogen sulfidefrom sulfate-rich water. Sufficient moisture must bepresent to prevent the desiccation of the bacteria. Theremust be adequate supplies of hydrogen sulfide, carbondioxide, nitrogen compounds, and oxygen. In addition,soluble compounds of phosphorus, iron, and other traceelements must be present in the moisture film.
Newly made concrete has a strongly alkaline surfacewith a pH of about 12. No species of sulfur bacteria canlive in such a stroug alkaline environment. Therefore, theconcrete is temporarily free from bacterially inducedcorrosion. Natural carbonation of the free lime by thecarbon dioxide in the air slowly drops the pH of theconcrete surface to 9 or less. At this level of alkalinity,the sulfur bacteria Thiobacillus thioparus, using hydrogensulfide as the substrate, generate thiosulfuric and poly-thionic acid. The pH of the surface moisture steadily de-clines, and at a pH of about 5, Thiobacillus concretivorusbegins to proliferate and produce high concentrations ofsulfuric acid, dropping the pH to a level of 2 or less. Thedestructive mechanism in the corrosion of the concreteis the aggressive effect of the sulfate ions on the calciumaluminates in the cement paste.
The main concrete corrosion problem in a sewer,therefore, is chemical attack by this sulfuric acid whichaccumulates in the crown of the sewer. Information isavailable which may enable the designer to design, con-struct, and operate a sewer so that the development ofsulfuric acid is reduced (Pomeroy 1974, ASCE-WPCFJoint Task Force 1982; ACPA 1981).
PART 2-CONTROL OF EROSIONCHAPTER 5--CONTROL OF CAVITATION
5.1-Hydraulic design principlesIn Chapter 2, Section 2.2, the cavitation index u was
defined by Eq. (2-l). When the value of u at which cavi-tation damage begins is known, a designer can calculatevelocity and pressure combinations that will avoidtrouble. To produce a safe design, the object is to assurethat the actual operating pressures and velocities willproduce a value of u greater than the value at whichdamage begins.
A good way to avoid cavitation erosion is to make ularge by keeping the pressurepO high, and the velocity volow. For example, deeply submerged baffle piers in a stil-ling basin downstream from a low spillway are unlikely tobe damaged by cavitation because both of these condi-tions are satisfied. This situation is illustrated in Fig. 5.1.The following example illustrates how u is calculated forthis case. From model studies, the mean prototype velo-
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES
city at 0, immediately upstream from the baffle block, isfound to be 30 ft/sec (9.1 m/sec), and the “minimum” pro-totype gage pressure, exceeded 90 percent of the time, is7.1 psi (49 kPa). The barometric pressure for the proto-type location is estimated to be 13.9 psi (95.8 kPa), sothat the absolute pressure at 0, 6.6 ft (2.0 m) aboveLocation 1, becomes
PO = 7.1 + 13.9 - (6.6 x 62.4) = 18.1 psi144 in?fi2 ’
pV = 0.3 psi
= 1.94 UWe2P l -ft
zc = 20
it follows that
~ = (18.1 - 0.3)( 144 in.2/ft2)(32.2 j&se~) = 2.9.
In SI units
2p. = 49 + 95.8 -
(2.0 x 9.a&@
Then, given that pv = 2.1 kPa, p = lo3 kg/m3, and zC =%
o = (125 - 2.1)(1000) _ = 2.9_’ - . .
This value of 0 is well above the accepted damagevalue of 2.3 for this shape of sharp-edged pier (Galperinet al. 1977). Hence, cavitation damage is unlikely in theprototype.
A second, equally effective procedure to avoid cavi-tation is to use boundary shapes and tolerances charac-terized by low values of GT for incipient damage. Forexample, a carefully designed gate slot, with an offset androunded downstream corner, may have a damage 0 aslow as 0.2. Unfortunately, the lowest value of a adesigner can use may be fixed by unintentional surfaceimperfections in concrete, the need for small abrupt ex-pansions in flow passages, or the likelihood that vorticeswill be generated by obstructions such as partially opensluice gates. To be realistic, one may have to expectboundary geometry that will cause cavitation damage, ifCJ drops below about 1.2.
A third choice, often inevitable, is to expect cavities toform at predetermined locations. In this case, the de-signer may: a) supply air to the flow, or b) use damage-resistant materials such as stainless steel, fiber-reinforcedconcrete, or polymer concrete systems.
Using damage-resistant materials will not eliminatedamage, but may extend the useful life of a surface. Thisalternative is particularly attractive, for example, forconstructing or repairing outlet works that will be usedinfrequently or abandoned after their purpose has beenserved.
In any case, values of CT at which cavitation erosionbegins are needed for all sorts of boundary geometries.Sometimes critical values of 0 may be estimated bytheory, but they usually come from model or prototypetests.
Fig. 5.1-Baffle block downstream from a low spillway
5.2-Cavitation indexes for damage and construction tol-erances
Fig. 5.2 lists a few values of 0 at which cavitation begins
Structure or Irregularity d References
Sudden expansion in tunnel
Russe 1 and Ball 1967Rouse and Jezdinsky 1966
Baffle blocks 1.4 & Galperin et al. 19772.3
Gates and gate slots 0.2 to Galperin et al. 19773.0 Ball 1959
Abraded concrete3/4 in. max. depthof roughness
0.6 Ball 1976
0.2 Ball 1976Arndt 1977Falvey 1982
Y////Y// */&/ '//I// 1.6
Yo- $'a 6mm
*Unusual definition of u
Fig. 5.2-Values of 0 at beginning of cavitation damage
210R-10 ACI COMMITTEE REPORT
and the references from which these values came. A de-signer should not use these numbers without studying thereferences. Some reasons for this are:
a. The exact geometry and test circumstances must beunderstood.
b. Authors use different locations for determining thereference parameters of Eq. (2-l). However, the generalform of Eq. (2-l) is accepted by practitioners in the field.
c. Similitude in the model is difficult to achieve.Many of the essential details involved in the original
references are explained in Hamilton (1983 and 1984)which deals with the examples in Fig. 5.2.
The values of u listed in Fig. 5.2 show the importanceof good formwork and concrete finishing. For example,a 1/4-in. (6-mm) offset into the flow which could becaused by mismatched forms has a u of 1.6, whereas a1:40 chamfer has a u only one-eighth this large. By thedefinition of u, the allowable velocity past the chamferwould be v/s times the allowable velocity past the offsetif p. - pV were the same in both cases. Thus, on a spill-way or chute where p0 - p, might be 17.4 psi (120 kPa),damage would begin behind the offset when the localvelocity reached 40 ft/sec (12 m/sec), but the flow pastthe chamfer would cause no trouble until the velocityreached about 113 ft/sec (35 m/sec).
When forms are required, as on walls, ceilings, andsteep slopes, skilled workmen may produce a nearlysmooth and only slightly wavy surface for which u may beas low as 0.4. Using the precedingpo -pv gives a damagevelocity of 80 ft/sec (24 m/sec). A u value of 0.2, onwhich the 113 ft/sec (35 m/sec) is based, may be achievedon plane, nearly horizontal surfaces by using a stiffscreed controlled by steel wheels running on rails andhand floating and troweling.
Construction tolerances should be included in all con-tract documents. These establish permissible variation indimension and location giving both the designer and thecontractor parameters within which the work is to be per-formed. ACI 117 provides guidance in establishing practi-cal tolerances. It is sometimes necessary that the specifi-cations for concrete surfaces in high-velocity flow areas,or more specifically, areas characterized by low values ofu, be even more demanding. However, achieving morerestrictive tolerances for hydraulic surfaces than thoserecommended by ACI 117 can become very costly oreven impractical. The final specification requirementsrequire judgment on the part of the designer (Schrader,1983).
Joints can cause problems in meeting tolerances, evenwith the best workmanship. Some designers prefer to sawand break out areas where small offsets occur rather thanto grind the offsets that are outside the specification. Thetrough or hole is then patched and hand finished in aneffort to produce a surface more resistant to erosion thana ground surface would be. In some cases grinding toachieve alignment and smoothness is adequate. However,to help prevent the occurrence of aggregate popouts, ageneral rule of thumb is to limit the depth of grinding to
one-half the maximum diameter of the coarse aggregate.Ground surfaces may also be protected by applying alow-viscosity, penetrating phenol epoxy-resin sealer(Borden et al. 1971). However, the smooth polished tex-ture of the ground surface or the smoothness of a resinsealer creates a different boundary condition which mayaffect the flow characteristics. Cavitation damage hasbeen observed downstream of such conditions in highvelocity flow areas [in excess of 80 ft/sec (24 m/sec) ]where there was no change in geometry or shape (Corpsof Engineers, 1939).
The difficulty of achieving a near-perfect surface andthe doubt that such a surface would remain smoothduring years of use have led to designs that permit theintroduction of air into the water to cushion the collapseof cavities when low pressures and high velocities prevail.
5.3-Using aeration to control damageLaboratory and field tests have shown that surface ir-
regularities will not cause cavitation damage if the air-water ratio in the layers of water near the solid boundaryis about 8 percent by volume. The air in the water shouldbe distributed rather uniformly in small bubbles.
When calculations show that flow without aeration islikely to cause damage, or when damage to a structurehas occurred and aeration appears to be a remedy, theproblem is dual: a) the air must be introduced into theflowing water and b) a portion of that air must remainnear the flow/concrete boundary where it will be useful.
The migration of air bubbles involves two principles:a) bubbles in water move in a direction of decreasingwater pressure, and b) turbulence disperses bubbles fromregions of high air concentration toward regions of lowconcentration.
Careful attention must be given to the motion ofbubbles due to pressure gradients. A flow of water sur-rounded by atmospheric pressure is called a free jet. Ina free jet, there are no gradients except possibly weaklocal ones generated by residual turbulence, and thebubbles move with the water. There is no buoyant force.On a vertical curve that is convex, the bubble motionmay have a component toward the bottom. In a flipbucket, which is concave, the bottom pressure is largeand the bubbles move rapidly toward the free surface.
When aeration is required, air usually must be intro-duced at the bottom of the flow. These bubbles graduallymove away from the floor in spite of the tendency forturbulent dispersion to hold them down. At the pointwhere insufficient air is in the flow to protect theconcrete from damage, a subsequent source of bottom airmust be provided.
Aeration data measured on Bratsk Dam in theC.S.I.R. (formerly the U.S.S.R), which has a spillwayabout 295 ft (90 m) high and an aeration device, havebeen discussed by Semenkov and Lentyaev (1973) (SeeTable 5.1). Downstream from the aeration ramp, mea-surements showed that the air-water ratio in a 6-in.(150-mm) layer next to the concrete declined from 85 to
35 percent as the mixture flowed down the spillway a dis-tance of 174 ft (53 m). If one assumes an exponentialtype of decay, the loss per foot was a little less than 2percent of the local air-water ratio.
It is usually not feasible to supply air to flowing waterby pumping or compressing the air because the volumesinvolved are too large. Instead, the flow is projected froma ramp or step as a free jet, and the water introduces airat the air-water interfaces. Then the turbulence withinthe jet disperses the air entrained at the interfaces intothe main body of the jet. Fig. 5.3 shows typical aerationramps for introducing air into the flow (Wei and De-Fazio 1982).
To judge whether sufficient air will remain adjacent tothe floor of a spillway, the amount of air that a turbulentjet will entrain must be estimated. The following equa-tion for entrainment by the lower surface has been pro-posed (Hamilton 1983 and 1984)
4a = lxve (5-2)
in which qa = volume rate of air entrainment per unit
width of jetcoefficientaverage jet velocity at midpoint of trajec-torylength of air space between the jet andthe spillway floor.
Model and prototype measurements indicate that thevalue of the coefficient Q! lies between 0.01 and 0.04,depending upon velocity and upstream roughness.
The length of cavity 4? (Fig. 5.3) is difficult to measurein prototypes and large models. Instead, the upper andlower profiles of the nappe can be estimated from two-dimensional irrotational flow theory. One method is touse a finite element technique for calculating nappetrajectories.
As indicated above, ramps and down-steps are used toinduce the flow in a spillway or tunnel to spring freefrom the floor. A ramp is a wedge anchored to or inte-gral with the floor and usually spans the tunnel or spill-way bay. Ramps vary in length from 3 to 9 ft (1 to 3 m).Wall and corner wedges and wall offsets away from theflow also are used to cause the water to leave the sidesof a conduit. The objective is to provide a sudden expan-sion of the solid boundaries. Such devices, often referredto as aerators, are visually depicted in Fig. 5.4 and 5.5.(See also Ball 1959, DeFazio and Wei 1983, and Russelland Ball 1967.)
Air is allowed to flow into a cavity beside or under ajet by providing passages as simple as the layout of theproject will permit. Sometimes the required rates of air-flow are enormous. For example, a cavity underneath aspillway nappe 49 ft (15 m) wide could entrain 5160ft3/sec (146 m3/sec) of air. A single passageway at least6.6 ft (2.0 m) in diameter would be needed to supply thisamount.
Although offsets, slots, and ramps in conduits can in-troduce air into ‘high-velocity flow to effectively controlcavitation, if improperly designed they can accentuate thecavitation problem. For this reason, it is advisable to con-duct physical hydraulic model studies to ensure the ade-quacy of a proposed aeration device.
Table 5.1-Examples of use of air to prevent cavitationdamage
Structure or description
Palisades Dam outlet sluices
Yellowtail Dam spillway tunnel
Glen Canyon Dam spillwaytunnel
Ust-Ilim Dam spillway
Bratsk Dam spillway
Foz do Areia spillway
Beichley and Ring, 1975
Borden et al., 1971,Colgate 1971
Burgi, Moyes, and Gamble,1984
Qskolkov and Semenkov,1973
Semenkov and Lentyaev,1973
Pinto et al., 1982
Galperin et al., 1977
Hamilton, 1983 and 1984,Quintela, 1980
Fig. 5.3-Aeration ramps at King Talal Spillway
1.6 f t
EL. 304.1 f t
(92 70 m)
E L . 3 0 1 . 7 f t
210R-12 ACI COMMITTEE REPORT
. . . . . . . . . _ . .
. . . . . . . . . . . . .
Fig. 5.4-Types of aerators (from Vischer, Volkart, andSiegen thaler, 1982)
P I E R I N F L O W
S L O T I N S I D E W A L L
O F F S E T S I D E W A L L
D U C T T H R O U G H S I D E W A L L
D U C T U N D E R R A M P
D U C T U N D E R O F F S E T
R A M P O N S I D E W A L L
Fig. 5.5-Air supply to aerators (from Falvey, 1990)
5.4-Fatigue caused by vibrationIn concrete, flexural fatigue is normally thought of in
terms of beams bending under repeated relatively highamplitudes and low-frequency loads. A mass of concreteat the surface of an outlet or spillway ordinarily does notbend, but it does vibrate. In this case, the deformation isthree-dimensional with low amplitude and high frequen-cy. For instance, at McNary Dam the viiration was mea-sured as 0.00002 in. (0.00051 mm) and 150 cycles persecond (cps) for the transverse direction. Unfortunately,there are no reported studies of concrete fatigue causedby vibration.
A vibration test for concrete and epoxy/polymermaterials is needed. Data from such a test would be use-ful for evaluating various construction and repair mater-ials. A standard test has been developed for small sam-ples of homogeneous materials which viirates the sampleat 20,000 cps and 0.002 in. (0.051 mm) amplitude whileit is submerged in the fluid. Stilling basin floors, walls,and outlets are essentially full-scale tests of the sametype.
5.5-MaterialsAlthough proper material selection can increase the
cavitation resistance of concrete, the only totally effectivesolution is to reduce or eliminate the factors that triggercavitation, because even the strongest materials cannotwithstand the forces of cavitation indefinitely. The dif-ficulty is that in the repair of damaged structures, thereduction or elimination of cavitation may be very diffi-cult and costly. The next best solution is to replace thedamaged concrete with more erosion-resistant materials.
In areas of new design where cavitation is expected tooccur, designers may include the higher quality materialsduring the initial construction or include provisions forsubsequent repairs in service. For example, in many in-stallations, stainless steel liners are installed on theconcrete perimeter downstream of slide gates to resistthe damaging effects of cavitation. These liners, althoughquite durable, may pit and eventually have to be re-placed.
The cavitation resistance of concrete where abrasionis not a factor can be increased by using a properlydesigned low water-cement ratio, high-strength concrete.The use of aggregate no larger than 1% in. (38 mm)nominal maximum size is recommended, and the use ofwater-reducing admixtures and chilled concrete hasproven beneficial. Hard, dense aggregate and good bondbetween aggregate and mortar are essential to achievingincreased cavitation resistance.
Cavitation-damaged areas have been successfully re-paired using steel fiber reinforced concrete (ICOLD1988). This material exhibits good impact resistancenecessary to resist the many tiny point loads and appearsto assist in arresting cracking and disintegration of theconcrete matrix. The use of polymers as a matrix binderor a surface binder has also been found to improve sub-stantially the cavitation resistance of both conventional
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES
0 TEST SLAB NO. 1 - CONVENTIONAL CONCRETE - Cement 600 lb/& (356 kg/m?; MSA 1 ‘h’ (38 mm)0 TEST SLAB NO. 2 - STEEL FRC - Cement 690 lb/yd3 (409 kg/m3); MSA ;A* (1 9 mm)l TEST SLAB NO. 3 - POLYMERIZED CONVENTIONAL - Cement 600 lb/y& (356 kg/m3); MSA 1 ‘h’ (38 mm)H TEST SLAB NO. 4 - POLYMERIZED FRC - C ement 690 Ib/yd3 (409 kg/m3); MSA W (19 mm)
Test Time, hr
MSA- Maximum Size aggregate
Fig. 5.6-Erosion depth versus time, Tarbela Dam concrete mixtures (from Houghton, Borge, and Paxton, 1978)
and fiber-reinforced concrete (Schrader 1978 and 1983b).Some coatings, such as neoprene or polyurethane,
have effectively reduced cavitation damage to concrete,but since near-perfect adhesion to the concrete is man-datory, the use of such coatings is not common. Oncethere is a tear or a chip in the coating, the entire coatingis soon peeled off.
5.6-Materials testingBecause of the massive size of most hydraulic struc-
tures, full-scale prototype testing is usually not possible.Model testing can identify many potential problem areas,but determining the ultimate effect of hydraulic forces onthe structure requires some judgment. In some cases, itis desirable to evaluate a material after it has been sub-jected for a reasonable period of time to flows of a mag-nitude approaching that expected during operation of thefacility.
The U.S. Army Corps of Engineers has evaluated ero-sion resistance of materials at the Detroit Dam (Oregon)High Head Erosion test flume (Houghton, Borge, andPaxton 1978). Erosion testing at the facility consists ofpreparing test slabs 21 in. (530 mm) wide by 10 ft (3 m)long using the desired material, coating, or overlay. High-velocity water, in excess of 80 ft/sec (24 m/sec), is passedover the slabs for various durations, and the performanceof the material is then evaluated. Cavitation erosion re-sistance is studied by embedding small obstacles in thetest slabs which protrude into the flow (Fig. 2.5).
Materials and coating systems evaluated for TarbelaDam repairs, were tested at the Detroit Dam facility.They included various concrete mixes, FRC, roller-com-pacted concrete, polymer-impregnated concrete, polymer-impregnated FRC, and several concrete coatings (Hough-
ton, Borge, and Paxton 1978). Fig. 5.6 shows the perfor-mance of several of these materials subjected to flowswith velocities of 120 ft/sec (37 m/sec).
5.7-Construction practicesConstruction practices are of paramount importance
when hydraulic surfaces may be exposed to high-velocityflow, particularly if aeration devices are not incorporatedin design. Such surfaces must be as smooth as can bepractically obtained (Schrader 1983b). Surface imperfec-tions and deficiencies have been known to cause cavita-tion damage at flow velocities as low as 26 ft/sec (8m/sec). Offsets no greater than % in. (3 mm) in heighthave been known to cause cavitation damage at flow vel-ocities as low as 82 ft/sec (25 m/sec). Patching repairsimproperly made at the time of construction have beenknown to fail under the stress of water flow or for otherreasons, thereby providing the surface imperfectionswhich triggered cavitation damage to the concrete fartherdownstream. This phenomenon occurred in the high headspillway tunnel at Yellowtail Dam, Montana, ultimatelyresulting in major cavitation and structural damage to theconcrete lining (Borden et al. 1971; Colgate 1971). Ac-cordingly, good construction practices as recommendedin ACI 117, ACI 302.1R, ACI 304, ACI 308, ACI 309,and ACI 347 should be maintained both for new con-struction and repair. Formed and unformed surfacesshould be carefully checked during each constructionoperation to confirm that they are within specifictolerances.
If the potential for cavitation damage exists, careshould be taken in placing the reinforcement. The barsclosest to the surface should be placed parallel to thedirection of flow so as to offer the least resistance to flow
210R-14 ACI COMMITTEE REPORT
in the event that erosion reaches the depth of thereinforcement. Extensive damage has been experiencedwhere the reinforcement near the surface is normal tothe direction of flow.
Where possible, transverse joints in concrete conduitsor chutes should be minimized. These joints are generallyin a location where the greatest problem exists in main-taining a continuously smooth hydraulic surface. Oneconstruction technique which has proven satisfactory inplacement of reasonably smooth hydraulic surfaces is thetraveling slipform screed. This technique can be appliedto tunnel inverts and to spillway chute slabs. Informationon the slipform screed can be found in Hurd (1979).
Proper curing of these surfaces is essential, since thedevelopment of surface hardness improves cavitation re-sistance.
CHAPTER 6-CONTROL OFABRASION EROSION
6.1-Hydraulic considerationsUnder appropriate flow conditions and transport of
debris, all of the construction materials currently beingused in hydraulic structures are to some degree suscep-tible to abrasion. While improvements in materialsshould reduce the rate of damage, these alone will notsolve the problem. Until the adverse hydraulic conditionswhich can cause abrasion erosion damage are minimizedor eliminated, it is extremely difficult for any of theconstruction materials currently being used to perform inthe desired manner. Prior to construction or repair ofmajor structures, hydraulic model studies of the structureshould be conducted to identify potential causes of ero-sion damage and evaluate the effectiveness of variousmodifications in eliminating those undesirable hydraulicconditions. If the model test results indicate it is im-practical to eliminate the undesirable hydraulic condi-tions, provisions should be made in design to minimizefuture damage. For example, good design practicesshould consider the following measures in the construc-tion or repair of stilling basins:
a. Include provisions such as debris traps or lowdivision walls to minimize circulation of debris.
b. Avoid use of baffles which are connected to stillingbasin walls. Alternatively, considering their susceptibilityto erosion, avoid use of appurtenances such as chuteblocks and baffles altogether when the design makes thispossible.
c. Use model tests for design and detailing of the ter-minus of the stilling basin and the exit channel, so as tomaximize flushing of the stilling basin and to minimizechances of debris from the exit channel entering thebasin.
Maintain balanced flows into the basins of existingstructures, using all gates, to avoid discharge conditionswhere flow separation and eddy action are prevalent.Substantial discharges that can provide a good hydraulic
jump without creating eddy action should be releasedperiodically in an attempt to flush debris from the stillingbasin. Guidance as to discharge and tailwater relationsrequired for flushing should be developed through modelor prototype tests, or both. Periodic inspections shouldbe required to determine the presence of debris in thestilling basin and the extent of erosion. If the debriscannot be removed by flushing operations, water releasesshould be shut down and the basin cleaned by othermeans.
6.2-Materials evaluationMaterials, mixtures, and construction practices should
be evaluated prior to use in hydraulic structures sub-jcctcd to abrasion-erosion damage. ASTM C1138 coversa procedure for determining the relative resistance ofconcrete to abrasion under water. This procedure simu-lates the abrasive action of waterborne particles (silt,sand, gravel, and other solid objects). This procedure isa slightly modified version of the test method (CRD-C63) developed by the U.S. Army Corps of Engineers. Thedevelopment of the test procedure and data from testson a wide variety of materials and techniques have beendescribed by Liu (1980).
6.3-MaterialsA number of materials and techniques have been used
in the construction and repair of structures subjected toabrasion erosion damage, with varying degrees of success.The degree of success is inversely proportional to thedegree of exposure to those conditions conducive to ero-sion damage (McDonald 1980). No single material hasshown consistently? superior performance when comparedto others. Improvements in materials are expected toreduce the rate of concrete damage due to abrasionerosion. The following factors should be considered whenselecting abrasion-resistant materials.
Abrasion-resistant concrete should include the largestmaximum size aggregate particle, the maximum amountof the hardest available coarse aggregate and the lowestpractical water-cementitious material ratio. The abra-sion-erosion resistance of concrete containing chert ag-gregate has been shown to be approximately twice that ofconcrete containing limestone (Fig. 6.1). Given a good,hard aggregate, any practice that produces a strongerpaste structure will increase abrasion-erosion resistance.In some cases where hard aggregate was not available,high-range water-reducing admixtures and silica fumehave been used to develop very strong concrete-that is,concrete with a compressive strength of about 15,000 psi(100 MPa)-and to overcome problems with unsatisfac-tory aggregate (Holland 1983). Apparently, at these highcompressive strengths, the hardened cement pasteassumes a greater role in resisting abrasion-erosiondamage and the aggregate quality becomes correspon-dingly less important.
Concrete, when producedwith shrinkage-compensatingcement, and when properly proportioned and cured, has
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 210R-15
an abrasion resistance from 30 to 40 percent higher thanportland cement concrete of comparable mixture propor-tions, [ACI 223 (1970) and Klieger and Greening (1969)].
Steel fiber-reinforced concrete typically has more pasteand mortar per unit volume of concrete, and thereforeless coarse aggregate than comparable conventional con-crete. Consequently, fiber-reinforced concrete would beexpected to have a lower resistance to abrasion-erosioncompared to conventional concrete. In laboratory tests,the abrasion loss of a range of fiber-reinforced concretemixtures was consistently higher than that of conven-tional concrete mixtures with the same water-cementratio and aggregate type (Liu and McDonald, 1981).However, the improved impact strength of fiber-rein-forced concrete (Schrader, 1981) may be expected toreduce concrete spalling where large debris is beingtransported by high velocity flow (ACI 544.1R, 1982).
The abrasion-erosion resistance of vacuum-treatedconcrete, polymer concrete, polymer-impregnated con-crete, and polymer-portland cement concrete is signi-ficantly superior to that of comparable conventionalconcrete. This is attributed to a stronger cement matrix.The increased costs associated with materials, production,and placing of these and any other special concretes incomparison with conventional concrete should be con-sidered during the evaluation process.
Several types of surface coatings have exhibited goodabrasion-erosion resistance in laboratory tests. Theseinclude polyurethanes, epoxy-resin mortar, furan-resinmortar, acrylic mortar, and iron-aggregate toppings.Problems in field application of surface coatings havebeen reported (McDonald 1980). These have been dueprimarily to improper surface preparation or thermalincompatibility between coatings and concrete. Morerecently, formulations have been developed which havecoefficients of thermal expansion more similar to that ofthe concrete substrate.
- LIMESTONE- - QUARTZITE -- - - TRAP ROCK- - - - CHERT
040.3 0.4 O S 0.6 0 7
Water -Cement Ra t i o
Fig. 6.1-Relationshipsabrasion-erosion loss
between water-cement ratio and
CHAPTER 7-CONTROL OF EROSIONBY CHEMICAL ATTACK
7.1-Control of erosion by mineral-free waterThe mild acid attack possible with pure water rarely
develops into deterioration that can cause severe struc-tural damage. Generally, the mineral-free water will leachmortar on surfaces exposed to this water. This can beseen on exposed surfaces and at joints and cracks in con-crete sections. As the surface mortar is leached from theconcrete, more coarse aggregate is exposed, which natur-ally decreases the amount of mortar exposed. With lessmortar exposed, less leaching occurs, and hence majorstructural problems do not usually result. The gradualerosion of the leached mortar can be minimized by useof special cements, addition of pozzolan to mixes, or useof a variety of protective coatings and sealants applied toconcrete surfaces (Tuthill 1966).
7.2-Control of erosion from bacterial actionThe process of sulfide generation in a sanitary sewer
when insufficient dissolved oxygen is present in thewastewater has been discussed and illustrated by anASCE-WPCF Joint Task Force (1982). This originalwork was performed by Pomeroy (1974). Continuingwork by Pomeroy and Parkhurst, 1977, produced a quan-titative method for sulfide prediction. Engineers involvedwith projects of this nature would be wise to also reviewthe recommendations set forth in the ACPA ConcretePipe Handbook.
Concrete conduits have served in sewer systems formany years without serious damage where the systemswere properly designed and operated. The minimum ade-quate velocity of flow in the sewer for the strength andtemperature of the sewage is usually 2 ft/sec (0.6 m/sec).Providing this velocity without excessive turbulence andproviding proper ventilation of the sewer will generallyprevent erosion by bacterial action. Turbulence is to beavoided because it is an H,S releasing mechanism.Where conditions are such that generation of H,S cannotbe totally eliminated by the design of the system, thenother means may be applied, such as:
1) using hydrogen peroxide or chlorine compounds toconvert the H,S (WPCF 1979).
a) Hz02 + H,S +--* 2H,O + Sb)(l) Cl, + H.,O ++ HOC1 + H+ + Cl-
(2) HOC1 + H,S ++ S + HCl + H,O (low pH)(3) S*- + 4C1, + 8OH- --*+ SO,*- + 8Cl + 4H,O
2) introducing compressed air to keep sewage freshand thereby prevent the development of the anaerobicenvironment;
3) using an acid-resistant pipe such as vitrified clay orpolyvinyl chloride (PVC) pipe;
4) using acid-resisting liners on the crown of sewers;and/or
210R-16 ACI COMMITTEE REPORT
5) increasing the concrete section to allow a sacrificialthickness based on predicted erosion rates.
Graphical methods have been published for deter-mining sulfide buildup in sanitary sewers, using thePomeroy-Parkhurst equations (Kienow et al. 1982).
Parker (1951) lists the following remedial measures forthe control of H,S attack in concrete sewers:
I. Reduction-potential-generation0 inflow reductionl partial purificationl chemical dosage to raise oxidation (but addition
of nitrates is impracticable)0 aerationl chlorinationl removal of slimes and silts* velocity increase
II. Emissionsl turbulence reductionl treatment with heavy metal salts (Cu, Fe, Zn)l treatment with alkalies0 full flow in sewer
III. HS fixation on concreteventilationperiodic wettinguse of resistant concreteammoniationuse of protective coatings
The designer faced with reducing bacterial actionshould be aware that a) chlorination may, under certaincircumstances, be illegal because it can produce trihal-omethane, a known carcinogen; and b) it may also be il-legal to add lead salts (which usually are the only cost-effective choice) or other heavy metal salts to wastewater.
Lining concrete pipe, walls, and conduit with polyvinylchloride (PVC) sheets is an effective method of protec-ting the concrete and reducing surface roughness. Thistechnique has been used commercially for many years.The designer should carefully determine whether thecomposition and thickness of PVC liners are appropriate
for each application.Further information on remedial measures for sanitary
sewer systems is available in U.S. Environmental Pro-tection Agency publication EPA/625/1-85/018 (1985).
7.3-Control of erosion by miscellaneous chemicalcauses
7.3.1 Acid environments-No portland cement con-crete, regardless of its other ingredients, will withstandattack from water of high acid concentration. Wherestrong acid corrosion is indicated, other constructionmaterials or an appropriate surface covering or treatmentshould be used. This may include applications of sulfur-concrete toppings, epoxy coatings, polymer impregnation,linseed-oil treatments, or other processes, each of whichaffects acid resistance differently. Replacement of a por-tion of the portland cement by a suitable amount of poz-zolan selected for that property can improve the resis-tance of concrete to weak acid attack. Also, limestone ordolomite aggregates have been found to be beneficial inextending the life of structures exposed to acid attack(Biczok 1967).
Deterioration similar to that which occurs in the crownof sewers has also occurred above water level in tunnelswhich drain lakes, the waters of which contain sulfur andother materials that are susceptible to the formation ofhydrogen sulfide by bacterial action.
PVC linings may also be used to control deteriorationand erosion of concrete in acid environments.
7.3.2 Alkali-aggregate reaction and chloride admixtures-Deterioration of concrete caused by alkali-aggregatereaction and by chloride admixtures in the concretemixture is not included in this discussion. TuthiIl (1966)and ACI 201.2R provide information on these topics.
7.3.3 Soils and ground waters-Sulfates of sodium,magnesium, and calcium frequently encountered in the“alkali” soils and ground waters of the western UnitedStates attack concrete aggressively. ACI 201.2R discussesthis in detail. Use of Type V sulfate-resisting cement,which is low in tricalcium aluminate (%A), is recom-mended whenever the sulfate in the water is within theranges shown for its use in Table 7.1. The subject ofdesigning a sulfate resistant concrete mixture is complex.It is generally agreed that limiting the %A content of thecement to the 3 to 5 percent range, as in a Type V ce-ment, is beneficial. But the same could be said of TypesI or II cements, where the C$A content is so restricted.Other issues are also important. There include: restrictingthe tetracalcium aluminoferrite content (C&F) to 10percent; providing air entrainment (an air entrained mixusing Type II cement can be more sulfate resistant thana non-air entrained mix using Type V cement); replacing20 to 30 percent of the cement content with a pozzolanor fly ash; and using a rich mix, with the water-cementratio restricted to 0.50. The use of shrinkage-compen-sating cements, made with Type II or Type V portlandcement clinker and adequately sulfated, produces con-crete having sulfate resistance equal to or greater than
Table 7.1-Recommended cement types to use in con-crete when mixing water contains sulfates
mg/l sulfate (asSO,) in water Cement type
150-1500 Type II, IP
1500-10,000 Type V, or Type I or II with a pozzolan whichhas been shown by test to provide comparablesulfate resistance when used in concrete, orType K shrinkage-compensating
10,000 or more Type V plus an approved pozzolan which hasbeen determined by tests to improve sulfateresistance when used in concrete along withType V
(from ACI 201.2R)
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 210R-17
portland cement made of the same type clinker (Mehtaand Polivka 1975). Table 7.1 lists the recommendedcement types for corresponding sulfate contents.
PART 3-MAINTENANCE AND REPAIROF EROSION
CHAPTER 8-PERIODIC INSPECTIONS ANDCORRECTIVE ACTION
8.1-GeneralThe regular, periodic inspection of completed and
operating hydraulic structures is extremely important.The observance of any erosion of concrete should be in-cluded in these inspections. The frequency of inspectionsis usually a function of use and evidence of distress. Theinspections provide a means of routinely examining struc-tural features as well as observing and discussing prob-lems needing remedial action. ACI 201.1R, ACI 207.3R,and U.S. Department of the Army publication EM-1110-2-2002 (1979) provide detailed instructions for conductingextensive investigations.
8.2- Inspection programThe inspection program must be tailored to the speci-
fic type of structure. The designers should provide inputto the program and identify items of primary and secon-dary importance. The actual inspection team should becomposed of qualified technical personnel who knowwhat to look for and can relate in common terminology.The size of the team is generally dependent on the num-ber of technical disciplines required. The program shouldbe established and monitored by an engineer who isexperienced in design, construction, and operation of theproject.
8.3-Inspection proceduresPrior to the on-site inspection, the team should thor-
oughly evaluate all available records, reports, and otherdocumentation on the condition of the structure andmaintenance and repair, and become familiar with previ-ous recommendations. Some of the more important ob-servations to make during an examination of hydraulicfacilities are:
a. Identifying structural cracking, spalling, and dis-placements within the water passage
b. Identifying surface irregularities1. Offset into or away from flow2. Abrupt curvature away from flow3. Abrupt slope away from flow4. Local slope changes along flow surface5. Void or transverse groove6. Roughened or damaged surfaces which give evi-
dence of cavitation or abrasion erosion7. Structural imperfections and calcite deposits8. Cracking, spalling, and rust stains from rein-
c. Inspecting gate slots, sills, and seals, includingidentification of offsets into the flow
d. Locating concrete erosion adjacent to embeddedsteel frames and steel liners and in downstream waterpassages
e. Finding vibration of gates and valves during oper-ation
f. Observing defective welded connections and thepitting and/or cavitation of steel items
g. Observing equipment operation and maintenanceh. Making surveys and taking cross sections to deter-
mine the extent of damagei. Investigating the condition of concrete by nonde-
structive methods or by core drilling and sampling, ifdistressed conditions warrant
j. Noting the nature and extent of debris in waterpassages
Observed conditions, the extent of the distress, andrecommendations for action should be recorded by theinspection team for future reference. High-qualityphotographs of deficiencies are extremely beneficial andprovide a permanent record which assists in identifyingslow progressive failures. A report should be written foreach inspection to record the condition of the projectand to justify funding for repairs.
8.4-Reporting and evaluationThe inspection report may vary from a formal publica-
tion to a trip report or letter report. The report shouldinclude the standard items: who, why, what, where, andwhen. A pre-established outline is usually of value. Aninspection checklist of deficiencies and subsequent cor-rective actions should be established from prior inspec-tions. Any special items of interest may be shown insketches or photos. The report should address existingand potential problems, and it should categorize thedeficiencies relative to the urgency of corrective actionand identify the extent of damage, probable cause ofdamage, and probable extent of damage if immediaterepairs are not made. It is extremely important that theowner or agency distribute the report in accordance withapplicable U.S. federal or state safety regulations.
When the inspection report indicates that remedialaction is required, the next step may be either a sup-plemental investigation or the actual corrective action.Deficiencies noted in the inspection should be evaluatedand categorized as to minor, major, or potentially cata-strophic. The scope of work should be defined as early aspossible in order to establish reliable budget estimates.Design for proper repair schemes sometimes requiresmodel tests, redesign of portions of the structure, andmaterials investigations. Each of these items requiresfunding through the owner’s program of operations. Themore details identified in the scope of work, the moreaccurate the cost estimate. Wherever possible, it is im-portant to correct the probable cause, so that the repairswill not have to be repeated in the near future.
210R-18 ACI COMMITTEE REPORT
CHAPTER 9-REPAIR METHODSAND MATERIALS
9.1-Design considerations9.1.1 General-It is desirable to eliminate the cause of
the erosion whenever possible; however, since this is notalways possible, a variety of materials and material com-binations is used for the repair of concrete. Some mater-ials are better suited for certain repairs, and judgmentshould be exercised in the selection of the proper mater-ial. Consideration also should be given to the time avail-able to make repairs, access points, logistics in materialsupply, ventilation, nature of the work, available equip-ment, and skill and experience of the local labor force.
Detailed descriptions of repair considerations and pro-cedures may be found in the U.S. Bureau of Reclama-tion’s Concrete Manual (1985).
9.1.2 Consideration of materials-A major factor whichis critical to the success of a repair is the relative volumechange between the repair material and the concrete sub-stratum. Many materials change volume as they initiallyset or gel, almost all change volume with changes inmoisture content, and all change volume with changes intemperature. If a repair material decreases sufficiently involume relative to the concrete, it will develop cracksperpendicular to the interface, generally at a spacingrelated to the repair depth. Shear and tensile stressesalso will develop at the interface with a maximum mag-nitude at the tip of each crack, and the stresses will cyclewith each temperature and moisture cycle. ASTM C 884evaluates a specific class of materials with respect totemperature change. Similar tests should be applied to allrepair materials.
Since differential volume change imposes stresses atan interface between a repair material and the concrete,suitable preparation of that interface is essential to thesuccess of the repair. Sound concrete may not be able toresist stresses imposed by a high volume change repairmaterial, whereas it may resist those imposed by a lowvolume change material. ACI 503R has recommendedthat the interface between concrete and epoxy patchesexhibit an absolute minimum tensile strength, by a spe-cific test method, of 100 psi (0.69 MPa).
Normal portland cement concrete is generally the leastexpensive replacement material and will most nearlymatch the characteristics of the in-place concrete withregard to temperature change. Normal concrete willalmost certainly be subject to an initial shrinkage relativeto the original concrete and possibly thermal stressesfrom heat of hydration if the depth of replacement issufficient to develop a significant temperature gradientwithin the repair.
The best way to minimize plastic and drying shrinkageis to minimize water content in the replacement concrete.Thus, stiff mixtures, with or without the incorporation ofpolymers or copolymers as a replacement for part of themix water, may be considered. Stiff mixtures may requirecareful use of bonding agents and be more difficult to
place and consolidate. It also may be difficult to con-solidate stiff mixtures around reinforcing steel. The useof polymers can improve the useability of the concrete,but also substantially increases material costs, maypresent additional handling hazards, and may requirespecial construction techniques.
9.2-Methods and materials9.2.1 Steel plating-Installing stainless steel liner plates
on concrete surfaces subject to cavitation erosion hasbeen a generally successful method of protecting the con-crete against cavitation erosion. Colgate’s (1977) studiesshow stainless steel to be about four times more resistantto cavitation damage than ordinary concrete. The cur-rently preferred stainless material is ASTM A 167,S30403 (formerly SS304L), from the standpoint of excel-lent corrosion and cavitation resistance, and weldability.The steel plates must be securely anchored in place andbe sufficiently stiff to minimize the effects of vibration.Vibration of the liner plate can lead to fracturing andeventual failure of the underlying concrete or failure ofthe anchors. Grouting behind the plates to prevent vibra-tion is recommended. Unfortunately, the steel platingmay hide early signs of concrete distress.
This repair method, like many others, treats only thesymptom of erosion and eventually, if the cavitation isnot reduced or eliminated, the steel itself may becomedamaged by pitting.
9.22 Dry-packed concrete-Use of dry-packed concreteis generally limited to applications where the materialcan be tamped into cavities which have a depth at leastas great as their width. These limited applications arenecessary because the material is friable until compactedin place by tamping or ramming. The low water contentof the dry-pack, combined with the density obtained bythe compaction process, gives a patch that will experiencevery little drying shrinkage and will have expansion pro-perties similar to the parent concrete.
Dry-pack should consist of one part cement to twoparts masonry sand (passing No. 16 screen) (1.18 mmsieve). Latexes and other special admixtures can be usedin the mixture when bonding or another special charac-teristic is desired. The consistency of the dry-pack mortarshould be such that when balled in the hand, the hand ismoist but not dirty. White cement can be blended withgray cement if appearance is important. The completedwork should be moist-cured, just as any concrete.
Dry-packed concrete repairs, as is true of all repairs,require care on the part of both designer and constructorto insure that the final product meets the intendeddesign. Properly made, dry-packed concrete repairs haveproven to be very satisfactory.
“Damp-pack,” a similar material discussed in U.S.Army Corps of Engineers Technical Report MRDL 2-74(1974) and the ACI Manual of Concrete Inspection(1981), can be sprayed onto existing concrete for repairof peeled areas and other shallow defects.
9.2.3 Fiber-reinforced concrete (FRC)-Conventional
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 210R-19
concrete typically performs poorly where the followingmaterial properties are important to the life of thestructure or its performance: fatigue strength, cavitationand abrasion-erosion resistance, impact strength, flexuralstrength and strain capacity, post-cracking load-carryingcapability, and high shear strength. FRC utilizes random-ly oriented discrete fiber reinforcement in the mixtureand offers a practical way of obtaining these propertiesfor most applications. ICOLD Bulletin 40A (1988) de-scribes its use in dams. FRC has been successfully usedin some erosion situations. There are examples whereFRC repairs have been resistant to the combined effectsof cavitation and abrasion erosion by large rock anddebris carried at high velocity. On the other hand,laboratory abrasion-erosion tests under conditions of lowvelocity carrying small-size particles have shown that theaddition of fibers may not be beneficial, and in fact maybe detrimental (Liu and McDonald 1981). ACI 544.1Rand ACI publication SP-81 provide additional informa-tion regarding the use of FRC.
9.2.4 Epoxy resins-Resins are natural or synthetic,solid or semisolid organic materials of high molecularweight. Epoxies are one type of resin. These materialsare typically used in preparation of special coatings oradhesives or as binders in epoxy-resin mortars and con-cretes. Several varieties of resin systems are routinelyused for the repair of concrete structures. ACI 503Rdescribes the properties, uses, preparations, mixtures,application, and handling requirements for epoxy resinsystems.
The most common use of epoxy compounds is inbonding adhesives. Epoxies will bond to most buildingmaterials, with the possible exception of some plastics.Typical applications include the bonding of fresh con-crete to existing concrete. Epoxies can be used also forbonding dry-pack material, fiber reinforced concrete,polymer concretes, and some latex-modified concretes tohardened concrete. Epoxy formulations have been devel-oped recently which will bond to damp concrete andeven bond to concrete under water. There are case his-tories of successful uses of these materials in hydraulicstructures. To help assure proper selection and use ofmaterials, consultation with product representatives isadvised before an epoxy is specified or procured. ASTMC 881 is a specification for epoxy bonding systems usefulin concrete repairs, and ACI 503.2 covers epoxy bondingin repair work.
Experience has shown that the application of epoxiescan create serious problems in areas of high-velocity flow.
If the finished surface has a very smooth or glassy tex-ture, flow at the boundary can be disrupted and mayhave the effect of a geometric irregularity which couldtrigger cavitation. This texture problem can be minimizedby using special finishing techniques and/or improving thesurface texture of the patch with sand. Sometimes thepatch can be too resistant to damage, with the result thatthe abutting original material erodes away, leaving anabrupt change in surface geometry and developing a con-
dition worse than the original damage.Epoxy mortars and epoxy concretes use epoxy resins
for binder material instead of portland cement. Thesematerials are ideal for repair of normally submergedconcrete, where ambient temperatures are relativeIyconstant. They are very expensive and can cause prob-lems as a result of their internal heat generation. Mixedresults have been observed in the epoxy-mortar repair oferosion of outlet surfaces, dentates, and baffle blocks(McDonald 1980). Depending on the epoxy formulation,the presence of moisture, either on the surface or ab-sorbed in the concrete, can be an important factor andaffect the success of the repair. ACI 503.4 is a speci-fication for epoxy mortar in repair work.
The concept of improving concrete by incorporatingthe epoxy directly into the mix was encouraged by thesuccessful latex modification of concrete (Murray andSchrader 1979). Several commercial products have beendeveloped and research is continuing. The epoxies gen-erally enhance the concrete’s resistance to freeze-thawspalling, chemical attack, and mechanical wear. Epoxy-modified concrete (Christie, McClain, and Melloan 1981)has a curing agent which is retarded by the water in themixture. As the water is used up by cement hydrationand drying, the epoxy resin begins to gel. Accordingly,the mixture will not become sticky until the portlandcement begins to set, and this greatly extends the “potlife” of the wet concrete. To date, these materials havelimited use in hydraulic structures.
9.2.5 Acrylics and other polymer systems-There arethree main ways in which polymers have been incorpor-ated into concrete to produce a material with improvedproperties as compared to conventional portland cementconcrete. These are polymer-impregnated concrete (PIC),polymer-portland cement concrete (PPCC), and polymerconcrete (PC).
Polymer-impregnated concrete (PIC) is a hydratedPortland-cement concrete that has been impregnated witha monomer which is subsequently polymerized in situ. Byeffectively case hardening the concrete surface, impreg-nation protects structures against the forces of cavitation(Schrader 1978) and abrasion erosion (Liu 1980). Thedepth of monomer penetration depends on the porosityof the concrete and the process and pressure underwhich the monomer is applied. In addition to noting thatthese materials are quite costly, the engineer is cautionedthat some monomer systems can be hazardous and thatmonomer systems require care in handling and should beapplied only by skilled workmen experienced in their use(DePuy 1975). Surface impregnation was used at Dwor-shak Dam in the repair of cavitation and abrasion ero-sion damage to the regulating outlet tunnels (Schraderand Kaden 1976a) and stilling basin (McDonald 1980,and Schrader and Kaden 1976b). High-head erosiontesting of PIC at Detroit Dam test facility has shownexcellent performance (U.S. Army Corps of Engineers1977).
Polymer portland cement concrete (PPCC) is made by
the addition of water-sipersible polymers directly intowet concrete mix. PPCC, compared to conventional con-crete, has higher strength, increased flexibility, improvedadhesion, superior abrasion and impact resistance, andusually better freeze-thaw performance and improveddurability. These properties can vary considerablydepending on the type of polymer being used. The mostcommonly used PPCC is latex-modified concrete (LMC).Latex is a dispersion of organic polymer particles inwater. Typically, the fine aggregate and cement factorsare higher for PPCC than for normal concrete.
Polymer concrete (PC) is a mixture of fine and coarseaggregate with a polymer used as the binder. This resultsin rapid-setting material with good chemical resistanceand exceptional bonding characteristics. So far, polymerconcrete has had limited use in large-scale repair of hy-draulic structures because of the expense of large vol-umes of polymer for binder. Thermal compatibility withthe parent concrete should be considered before usingthese materials.
Polymer concretes are finding application as concreterepair materials for patches and overlays, and as precastelements for repair of damaged surfaces (Fontana andBartholomew 1981; Scanlon 1981; Kuhlmann 1981; Bhar-gava 1981). Field test installations with precast PC havebeen made on parapet walls at Deadwood Dam, Idaho,and as a repair of cavitation and abrasion damage in thestilling basin of American Falls Dam.
ACI 548R and ACI SP-58, “Polymers in Concrete(1978),” provide an overview of the properties and use ofpolymers in concrete. Smoak (1985) has described poly-mer impregnation and polymer concrete repairs at GrandCoulee Dam.
9.2.6 Silica-fume concrete-Laboratory tests haveshown that the addition of an appropriate amount ofsilica fume and a high-range water-reducing admixture toa concrete mixture will greatly increase compressivestrength. This, in turn, increases abrasion-erosionresistance (Holland 1983, 1986a, 1986b). As a result ofthese tests, concretes containing silica fume were used bythe US Army Corps of Engineers to repair abrasion-erosion damage in the stilling basin at Kinzua Dam(Holland et al. 1986) and in the concrete lining of thelow-flow channel. Los Angeles River (Holland and Gut-schow 1987). Despite adverse exposure conditions, par-ticularly at Kinzua Dam, the silica fume concrete con-tinues to exhibit excellent resistance to abrasion erosion.
Silica fume offers potential for improving many prop-erties of concrete. However, the very high compressivestrength and resulting increase in abrasion-erosion re-sistance are particularly beneficial in repair of hydraulicstructures. Silica fume concrete should be considered inrepair of abrasion-erosion susceptible locations, parti-cularly in those areas where available aggregate mightnot otherwise be acceptable. Guidance on the use ofsilica fume in concrete is given in ACI 226 (1987).
9.2.7 Shotcretes-Shotcrete has been used extensivelyin the repair of hydraulic structures. This method permits
replacing concrete without the use of formwork, and therepair can be made in very restricted areas. Shotcrete,also known as pneumatically applied mortar, can be aneconomical alternative to other more conventional sys-tems of repair. ACI 506R provides guidance in the man-ufacture and application of shotcrete. In addition to con-ventional shotcrete, modified concretes such as fiber-reinforced shotcrete, polymer shotcrete, and silica fumeshotcrete have been applied by the air-blown or shotcretemethod.
9.2.8 Coatings--High-head erosion tests have beenconducted using both polyurethane and neoprene coat-ings (Houghton, Borge, and Paxton 1978). Both coatingsexhibited good resistance to abrasion and cavitation. Theproblem with flexible coatings like these is their bond tothe concrete surfaces. Once an edge or a portion of thecoating is torn from the surface, the entire coating can bepeeled off rather quickly by hydraulic force.
9.2.9 Preplaced-aggregate concrete-Preplaced-aggregateconcrete, also referred to as “prepacked concrete,” is usedin the repair of large cavities and inaccessible areas.Clean, well-graded coarse aggregate, generally of 0.5 to1.5 in. (12 to 38 mm) maximum size, is placed in theform. Neat cement grout or a sanded grout, with or with-out admixtures, is then pumped into the aggregate matrixthrough openings in the bottom of the forms or throughgrout pipes embedded in the aggregate. The grout isplaced under pressure, and pressure is maintained untilinitial set. Concrete placed by this method has a lowvolume change because of the point-to-point contact ofthe aggregate; there is high bond strength to top bars forthe same reason. The use of pozzolans, water-reducingadmixtures, and low water contents is recommended tofurther reduce shrinkage and thermal volume changes,while maintaining the fluidity required for the grout tocompletely fill the voids in the aggregate. ACI 304.1Rprovides details and guidance for the use of preplaced-aggregate concrete.
9.2.10 Pipe inserts--For repair of small-diameter pipes,many of the methods discussed in the previous sectionsof this report are not applicable. A common constructionpractice today is to obtain a jointless, structurally soundpipe-inside-a-pipe without excavating the existing un-sound pipe. One such method that has been used suc-cessfully is to insert a plastic pipe inside the deterioratedconcrete pipe and then fill the annular space between theconcrete and plastic liner with grout. With the properselection of material for the plastic liner pipe insert, thisrepair method can provide a sound, chemically resistantlining (U.S. Dept. of Housing and Urban Development1985, and U.S. Environmental Protection Agency 1983).
Another popular method is the installation of a resinsaturated fiberglass “hose” into the pipeline. The hose isinserted into the pipeline using water pressure. After in-stallation, the hose is filled with hot water to initiate thechemical reaction of the resin. The hardened resin formsa rigid pipe lining.
9.2.11 Linings-Tunnels, conduits, and pipes that have
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 21 OR-21
9.2.12 Aeration slots-The installation of an aerationslot is not only a consideration in the design of a newfacility but often a very appropriate remedial addition toa structure experiencing cavitation erosion damage.Structural restoration and the addition of aeration slotshas been used in the repair of several structures. SeeSection 5.3 for a more detailed discussion of this method.The addition of aeration slots will likely reduce the flowcapacity of the structure significantly because of theadded volume of entrained air.
surface damage due to abrasion erosion, bacterial action,or chemical/acid attack can be protected from furtherdamage with a non-bonded mechanically attached PVClining. Depending on the extent of the damage, somepatching of the concrete surface may be required beforeinstallation.
l0.1-Specified and/or recommended referencesThe documents of the various standards-producing
organizations referred to in this document are listedbelow with their serial designation.
American Concrete Institute117
Standard Specifications for Tolerance for Con-crete Construction and MaterialsGuide for Making a Condition Survey of Con-crete in ServiceGuide to Durable ConcretePractices for Evaluation of Concrete in ExistingMassive Structures for Service ConditionsStandard Practice for the Use of Shrinkage-Compensating ConcreteGuide for Concrete Floor and Slab Construc-tionGuide for Measuring, Mixing, Transporting,and Placing ConcreteStandard Practice for Curing ConcreteGuide for Consolidation of ConcreteGuide to Formwork for ConcreteUse of Epoxy Compounds with ConcreteStandard Specification for Bonding Plastic Con-crete to Hardened Concrete with a Multi-Com-ponent Epoxy AdhesiveStandard Specification for Repairing Concretewith Epoxy MortarsGuide to ShotcreteSpecification for Materials, Proportioning, andApplication of ShotcreteState-of-the-Art Report on Fiber ReinforcedConcreteMeasurement of Properties of Fiber ReinforcedConcreteGuide for Use of Polymers in Concrete
Society for Testing and MaterialsStandard Specification for Stainless and
C 150C 131
Heat-Resisting Chromium-Nickel Steel Plate,Sheet, and StripStandard Specification for Portland CementStandard Test Method for Resistance to Degra-dation o f Small-Size Coarse Aggregate by Ab-rasion and Impact in the Los Angeles MachineStandard Test Method for Abrasion Resistanceof Concrete by SandblastingStandard Test Method for Resistance to Degra-dation of Large-Size Coarse Aggregate by Ab-rasion and Impact in the Los Angeles MachineStandard Test Method for Abrasion Resistanceof Horizontal Concrete SurfacesStandard Specification for Epoxy-Resin-BaseBonding Systems for ConcreteStandard Test Method for Thermal Compatibil-ity Between Concrete and an Epoxy-ResinOverlayStandard Test Method for Abrasion Resistanceof Concrete (Underwater Method)
U.S. Army Corps of EngineersCRD-C 63-80 Test Method for Abrasion-Erosion Resis-
tance of Concrete (Underwater Method)
These publications may be obtained from the followingorganizations:
American Concrete InstituteP.O. Box 19150Detroit, MI 48219
ASTM1916 Race St.Philadelphia, PA 19103
U.S. Army Corps of EngineersU.S. Army Engineer Waterways Experiment StationVicksburg, MS 39180
10.2-Cited referencesACI Committee 226, “Silica Fume in Concrete,” ACI
Materials Journal, V. 84, No. 2, Mar.-Apr. 1987.ACI Manual of Concrete Inspection, SP-2, 7th Edition,
American Concrete Institute, Detroit, 1981, pp. 224-225.ACPA, Concrete Pipe Handbook, American Concrete
Pipe Association, Vienna, Va., 1980, 450 pp.ASCE-WPCF Joint Task Force, Gravity Sanitary Sewer
Design and Construction, ASCE Manuals and Reports onEngineering Practice No. 60, American Society of CivilEngineers, New York, 1982, pp. 47-66.
Arndt, Roger E.A., Apr. 1977, “Discussion of Cavita-tion from Surface Irregularities in High Velocity” byJames W. Ball, Proceedings, ASCE, V. 103, HY4, pp.469-472.
Arndt, R.E.A., “Recent Advances in Cavitation Re-search,” Advances in Hydroscience 12, Academic Press,
210R-22 ACI COMMITTEE REPORT
New York, 1981, pp. l-78.Ball, J., Oct. 1959, “Hydraulic Characteristics of Gate
Slots,” Proceedings, ASCE, V. 85, HYlO, pp. 81-113.Ball, James W., Sept. 1976, “Cavitation from Surface
Irregularities in High Velocity,” Proceedings, ASCE, V.102, HY9, pp. 1283-1297.
Beichley, Glenn L., and King, Danny L., July 1975,“Cavitation Control of Aeration of High-Velocity Jets,”Proceedings, ASCE, V. 101, HY7, pp. 829-846.
Bhargava, Jitendra K., “Polymer-Modified Concretefor Overlays: Strength and Deformation Characteristics,”Applications of Polymer Concrete, SP-69, American Con-crete Institute, Detroit, 1981, pp. 205-218.
Bi&k, Imre, Concrete Corrosion and Concrete Protec-tion, Chemical Publishing Co., New York, 1967, 543 pp.
Borden, R.C., et al., May 1971, “Documentation ofOperation, Damage, Repair and Testing of YellowtailDam Spillway,"Report No. REC-ERC-71-23, U.S. Bureauof Reclamation, Denver.
Burgi, P.H.; Moyes, B.M.; and Gamble, T.W., “Opera-tion of Glen Canyon Dam Spillways--Summer 1983,”Water for Resource Development, American Society ofCivil Engineers, New York, 1984.
Christie, Samuel H., III; McClain, Roland R.; andMelloan, James H., “Epoxy-Modified Portland CementConcrete,” Applications of Polymer Concrete, SP-69,American Concrete Institute, Detroit, 1981, pp. 155-167.
Colgate, D., Dec. 1971, “Hydraulic Model Studies ofAeration Devices for Yellowtail Dam Spillway Tunnel,”Report No. REC-ERC-71-47, U.S. Bureau of Reclama-tion, Denver.
Colgate, Donald, “Cavitation Damage in HydraulicStructures,” Wear of Materials, American Society ofMechanical Engineers, New York, 1977.
DeFazio, F.G., and Wei, C.Y., “Design of AerationDevices on Hydraulic Structures,” Frontiers in HydraulicEngineering, American Society of Civil Engineers, NewYork, 1983, pp. 426-431.
DePuy, G.W., June 1975, “Process Technology Devel-opments with Concrete Polymer Materials-A SummaryReport,” Report No. GR-4-75, U.S. Bureau of Recla-mation, Denver.
Falvey, H.T., Aug. 1982, “Predicting Cavitation inTunnel Spillways,” International Water Power and DamConstruction (Sutton), V. 34, No. 8, pp. 13-15.
Falvey, H.T., April 1990, “Cavitation in Chutes andSpillways,’ Engineering Monograph, No. 42, U.S. Bureauof Reclamation, Denver.
Fontana, Jack J., and Bartholomew, John, ‘Use ofConcrete Polymer Materials in the TransportationIndustry,” Applications of Polymer Concrete, SP-69,American Concrete Institute, Detroit, 1981, pp. 21-43.
Galperin, R.; Oskolkov, A.; Seminkov, V.; and Tse-drov, G., Cavitation in Hydraulic Structures, EnergiyaPublishing House, Moscow, 1977 (in Russian).
Hamilton, W.S., “Preventing Cavitation Damage toHydraulic Structures,” International Water Power and DamConstruction (Sutton), V. 35, NOV. 1983, pp. 40-43, V. 35,
Dec. 1983, pp. 48-53, and V. 36, Jan. 1984, pp. 42-45.Holland, Terence C., “Abrasion-Erosion Evaluation of
Concrete Mixtures for Stilling Basin Repairs, KinzuaDam, Pennsylvania,” Miscellaneous Paper No. SL-83-16,U.S. Army Engineer Waterways Experiment Station,Vicksburg, 1983.
Holland, T.C., Abrasion-Erosion Evaluation of Con-crete Mixtures for Repair of Low-Flow Channel, LosAngeles River,” Miscellaneous Paper SL-86-12, U.S. ArmyEngineer Waterways Experiment Station, Vicksburg,1986a.
Holland, T.C., “Abrasion-Erosion Evaluation of Con-crete Mixtures for Stilling Basin Repairs, Kinzua Dam,Pennsylvania,” Miscellaneous Paper SL-86-14, U.S. ArmyEngineer Waterways Experiment Station, Vicksburg,1986b.
Holland, T.C., and Gutschow, R.A., ‘Erosion Resis-tance with Silica-Fume Concrete,” Concrete International,V. 9, No. 3, American Concrete Institute, Detroit, 1987.
Holland, T.C., Krysa, A., Luther, M.D., and Liu, T.C.,“Use of Silica-Fume Concrete to Repair Erosion Damagein the Kinzua Dam Stilling Basin,” Fly Ash, Silica Fume,Slag, and Natural Pozzolans in Concrete, SP-91, V. 2,American Concrete Institute, Detroit, 1986.
Holland, Terence C.; Husbands, Tony B.; Buck, AlanD.; and Wong, G. Sam, “Concrete Deterioration in Spill-way Warm-Water Chute, Raystown Dam, Pennsylvania,”Miscellaneous Paper, No. SL-80-19, U.S. Army EngineerWaterways Experiment Station, Vicksburg, Dec. 1980,49pp.
Houghton, D.L.; Borge, O.E.; and Paxton, J.H., Dec.1978, “Cavitation Resistance of Some Special Concretes,”ACI Journal, Proceedings, V. 75, No. 12, pp. 664-667.
Hurd, M.K., Formwork for Concrete, SP-4,4th Edition,American Concrete Institute, Detroit, 1979, 464 pp.
ICOLD, “Fiber Reinforced Concrete,” Bulletin No.4OA, International Commission on Large Dams, Paris,1988.
ICOLD, Transactions, 4th International Congress onLarge Dams (New Delhi, 1951), International Commis-sion on Large Dams, Paris, 1951.
Jansen, Robert B., “Advanced Dam Engineering fordesign, Construction, and Rehabilitation,” Van NostrandReinhold, New York, 1988, pp. 609-721.
Kienow, Karl E.; Pomeroy, Richard E.; and Kienow,Kenneth K., Oct. 1982, “Prediction of Sulfide Buildup inSanitary Sewers,” Proceedings ASCE, V. 108, EE5, pp.941-956.
Klieger, P., and Greening, N.R., “Properties of Expan-sive Cement Concretes,” Proceedings, 5th InternationalSymposium on the Chemistry of Cement (Tokyo, 1968),Cement Association of Japan, Tokyo, 1969, pp. 439-456.
Knapp, R.T.; Daily, J.W.; and Hammitt, F.G., Cavi-tation, McGraw-Hill Book Co., New York, 1970, pp.41-45 and 239-240.
Kuhlmann, L.A., “Performance History of Latex-Modified Concrete Overlays,” Applications of PolymerConcrete, SP-69, American Concrete Institute, Detroit,
EROSION OF CONCRETE IN HYDRAULIC STRUCTURES 210R-23
1981, pp. 123-144.Liu, Tony C., “Maintenance and Preservation of Con-
crete Structures: Report 3, Abrasion-Erosion Resistanceof Concrete,” Technical Report No. C-78-4, U.S. ArmyEngineer Waterways Experiment Station, Vicksburg,1980.
Liu, T.C., and McDonald, J.E., “Abrasion-Erosion Re-sistance of Fiber-Reinforced Concrete,” Cement, Con-crete, and Aggregates, V. 3, No. 2, Winter 1981, pp. 93-100.
McDonald, James E., “Maintenance and Preservationof Concrete Structures: Report 2, Repair of ErosionDamaged Structures,” Technical Report No. C-78-4, U.S.Army Engineer Waterways Experiment Station, Vicks-burg, 1980.
Mehta, P.K., and Polivka, Milos, “Sulfate Resistance ofExpansive Cement Concretes,” Durability of Concrete, SP-47, American Concrete Institute, Detroit, 1975, pp. 367-379.
Murray, Myles A., and Schrader, Ernest K., July-Aug.1979, “Epoxy Concrete Overlays,” The Military Engineer,V. 71, No. 462, pp. 242-244.
Oskolkov, A., and Semenkov, V., Aug. 1979, ‘Experi-ence in Developing Methods for Preventing Cavitation inStructures for Excess Flow Release,” Gidrotekh Stroitel(Moscow), No. 8, pp. 11-15.
Parker, C.D., Dec. 1951, ‘Mechanics of Corrosion ofConcrete Sewers by Hydrogen Sulfide,’ Sewage and In-dustrial Wastes, V. 23, No. 12, pp. 1477-1485.
Pinto, N.L., et al., “Aeration at High Velocity Flows,”International Water Power and Dam Construction (Sutton),V. 34, No. 2, Feb. 1982, pp. 34-38, and No. 3, Mar. 1982,pp. 42-44.
Polymers in Concrete: International Symposium, SP-58,American Concrete Institute, Detroit, 1978, 426 pp.
Pomeroy, Richard D., and Parkhurst, John D., “TheForecasting of Sulfide Build-Up Rates in Sewers,”Progress in Water Technology, V. 9, 1977.
Pomeroy, R.D., Oct. 1974 Process Design Manual forSul f ide Control in Sanitary Sewerage Systems, EPA 625-1-7-005 and NTIS PB/260/479.
Quintela, A.C., Jan. 1980, ‘Flow Aeration to PreventCavitation Erosion,” International Water Power and DamConstruction (Sutton), V. 32, No. 1, pp. 17-22.
Rigdon, J.H., and Beardsley, C.W., Apr. 1958, “Corro-sion of Concrete by Autotrophes,” Corrosion, V. 14, No.4, pp. 60-62.
Rouse, H., Elementary Mechanics of Fluids, John Wiley& Sons, New York, 1946 (republished by Dover Publica-tions, Inc., New York, 1978), pp. 62, 84-85, and 235-238.
Rouse, Hunter, and Jezdinsky, Vladimir, May 1966,“Fluctuation of Pressure in Conduit Expansions,” Pro-ceedings, ASCE, V. 92, HY3, pp. 1-12.
Russell, Samuel O., and Ball, James W., July 1967,“Sudden-Enlargement Energy Dissipator for Mica Dam,”Proceedings, ASCE, V. 93, HY4, pp. 41-56.
Scanlon, John M., Jr., “Applications of ConcretePolymer Materials in Hydrotechnical Construction,” Ap-
plications of Polymer Concrete, SP-69, American ConcreteInstitute, Detroit, 1981, pp. 45-62.
Schrader, Ernest K., “The Use of Polymers in Con-crete to Resist Cavitation/Erosion Damage,” Proceedings,2nd International Congress on Polymers in Concrete,College of Engineering, University of Texas, Austin,1978, pp. 283-309.
Schrader, Ernest K., “Cavitation Resistance of Con-crete Structures,” Frontiers in Hydraulic Engineering,American Society of Civil Engineers, New York, 1983.
Schrader, Ernest K., and Kaden, Richard A., May-June 1976a, “Outlet Repairs at Dworshak Dam,” TheMilitary Engineer, V. 68, No. 443, pp. 254-259.
Schrader, Ernest K., and Kaden, Richard A., July-Aug.1976b, "Stilling Basin Repairs at Dworshak Dam’” TheMilitary Engineer, V. 68, No. 444, pp. 282-286.
Schrader, Ernest K., Mar.-Apr. 1981, “Impact Resis-tance and Test Procedure for Concrete,” ACI Journal, pp.141-146.
Semenkov, V., and Lentyaev, L., May 1973, "SpillwayDam with Aeration of Overflow,” Gidrotekhs Stroitel(Moscow), No. 5, pp. 16-20.
Smoak, W. Glenn, “Polymer Impregnation and Poly-mer Concrete Repairs at Grand Coulee Dam,” PolymerConcrete: Uses, Materials, and Properties, SP-89, AmericanConcrete Institute, Detroit, 1985, pp. 43-49.
Tullis, J. Paul, Nov. 1981, “Modeling Cavitation forClosed Conduit Flow,” Proceedings, ASCE, V. 107, HYll,pp. 1335-1349.
Tuthill, L.H., “Resistance to Chemical Attack,” Signi-ficance of Tests and Properties of Concrete and Concrete-Making Material, STP-169A, ASTM, Philadelphia, 1966,pp. 275-289.
U.S. Army Corps of Engineers, Jan. 1977, “Investiga-tion of Cavitation-Erosion Resistance of ConventionalSteel Fiber and Polymer Impregnated Concrete for Tar-bela Dam,” North Pacific Division Materials Laboratory,Troutdale, 29 pp.
U.S. Army Corps of Engineers, Mar. 1974, “Develop-ment of Equipment and Techniques for PneumaticApplication of Portland Cement Mortar in ShallowDefects,” Techical Report No. MRDL 2-74, MissouriRiver Division, Omaha.
U.S. Army Corps of Engineers, Sept. 1989, PeriodicInspection Report No. 9.
U.S. Bureau of Reclamation, Concrete Manual, 8thEdition, Denver, 1975, Revised 1981, 627 pp.
U.S. Department of Army, Maintenance and Repair ofConcrete and Concrete Structures, Publication NO.EM- 1110-2-2002, 1979.
U.S. Department of Housing and Urban Development,July 1985, Utility Infrastructure Rehabilitation Methods,Publication No. HUD-PDR-952(l), Chapter 5.
U.S. Environmental Protection Agency, Oct. 1983,Demonstration of Sewer Relining by the Insituform Process,Northbrook, Illinois, Publication No. EPA-600/2-83-064,Cincinnati.
U.S. Environmental Protection Agency, Oct. 1985, De-
210R-24 ACI COMMITTEE REPORT
sign Manual-Odor and Corrosion Control in SanitarySewerage Systems and Treatment Plants, Publication No.EPA/625/1-85/018, Cincinnati.
Vischer, D.; Volkart, P.; and Siegenthaler, A.,“Hydraulic Modelling of Air Slots in Open Chute Spill-ways,” Proceedings, International Conference on theHydraulic Modelling of Civil Engineering Structures,”British Hydromechanics Research Association, Bedford,1982.
Wagner, William E., Nov. 1967, “Glen Canyon DamDiversion Tunnel Outlets,” Proceedings, ASCE, V. 93,HY6, pp. 113-134.
Wei, C., and DeFazio, F., “Simulation of Free JetTrajectories for the Design of Aeration Devices onHydraulic Structures,” Proceedings, 4th InternationalConference on Finite Elements in Water Resources(Hanover, June 1982), Hampshire ComputationalMechanics Centre, Ashurst-Southampton, 1982.
Wetzel, R.G., Limnology, W.B. Saunders Co.,Philadelphia, 1975, p. 271.
WPCF, “Odor Control for Waste Water Facilities,”Manual of Practice No. 22, Water Pollution ControlFederation, Washington, D.C., 1979.
a = coefficiente = length of air space between the jet and the spill-
way floor, e’
PO = absolute pressure at a given Point 0, F/e2
P” = vapor pressure of water, F/e24a = volume rate of air entrainment per unit width of
qd = amount of air a turbulent jet will entrain alongits lower surface, e3/T
V = average jet velocity at midpoint of trajectory, 4/Tvo = average velocity at section 0, UT
2, = elevation of the vapor bubble, 4
ZO = elevation at centerline of pipe, 4Y = specific weight of water, F/e3
P = density of water, F@/@a = cavitation index
=c = value of cavitation index at which cavitation ini-tiates
l C = length, F =force,T=time
I 210R-93 was submitted to letter ballot of the committee and processed inordance with ACI standardization procedures.